Tuning the surface functionality of polyethylene glycol-modified graphene oxide/chitosan composite for efficient removal of dye

There has been a lot of attention on water pollution by dyes in recent years because of their serious toxicological implications on human health and the environment. Therefore, the current study presented a novel polyethylene glycol-functionalized graphene oxide/chitosan composite (PEG-GO/CS) to remove dyes from aqueous solutions. Several characterization techniques, such as SEM, TEM, FTIR, TGA/DTG, XRD, and XPS, were employed to correlate the structure–property relationship between the adsorption performance and PEG-GO/CS composites. Taguchi’s (L25) approach was used to optimize the batch adsorption process variables [pH, contact time, adsorbent dose, and initial concentration of methyl orange (MO)] for maximal adsorption capacity. pH = 2, contact time = 90 min, adsorbent dose = 10 mg/10 mL, and MO initial concentration = 200 mg/L were found to be optimal. The material has a maximum adsorption capacity of 271 mg/g for MO at room temperature. With the greatest R2 = 0.8930 values, the Langmuir isotherm model was shown to be the most appropriate. Compared to the pseudo-first-order model (R2 = 0.9685), the pseudo-second-order model (R2 = 0.9707) better fits the kinetic data. Electrostatic interactions were the dominant mechanism underlying MO sorption onto the PEG/GO-CS composite. The as-synthesized composite was reusable for up to three adsorption cycles. Thus, the PEG/GO-CS composite fabricated through a simple procedure may remove MO and other similar organic dyes in real contaminated water.


Characterization. Scanning electron microscope.
A field-emission scanning electron microscope (Philips SEM 515, Germany) was utilized in order to investigate the surface morphologies of as-prepared samples.The samples were covered with gold before the measurements, and then they were subjected to an accelerated voltage of 10 kV for observation.
Transmission electron microscopy.Transmission electron microscopy (TEM, JEM-2100, Japan) with an acceleration voltage of 80-200 kV was used to ascertain the structure and orientation of the synthesized composites.The samples were assessed at a magnification of 50-1,500,000, a spot resolution of 0.23 nm, and a lattice resolution of 0.14 nm.
X-ray photoelectron spectroscopy.Using an X-ray photoelectron spectrometer, the surface chemical compositions of the samples were examined (ThermoFisher ESCALAB 250 XI).AlKα, with a pass energy of 20 eV, served as the X-ray source (h = 1360 eV).The XPS chamber was under 300 W of power, and the pressure varied from 107 to 109 Pa.FTIR analysis.A Bruker Optik EQUINOX 55 spectrophotometer (Ettlingen, Germany) was used to analyze the Fourier Transformation Infrared (FTIR) spectra of samples over the wavenumber range of 4000-400 cm −1 .After cutting and mixing the samples with the potassium bromide, the samples were ground into a pellet, which was then kept at room temperature (23 °C).
XRD analysis.Powder XRD patterns of samples were analyzed using a Rigaku Ultima III X-ray diffractometer (Texas, USA).Using CuKα radiation with a wavelength of λ = 1.54056 as the source, the crystallization behavior configuration was scanned from a phase angle of 2θ = 5°-60° with a step size of 0.02°.Thermogravimetric analysis.A thermogravimetric analyzer (TGA/DSC1, Mettler-Toledo Instruments Co., Ltd.Shanghai, China) was used to investigate the thermal behaviour of samples.The curves were measured from 30 to 800 °C at a constant heating rate of 10 °C/min in a nitrogen environment (flow rate of 50 mL/min).
Zeta potential.The adsorbent's surface charge through zeta potential was measured employing a Nano series ZETA SIZER (PHENOM-WORLD, Netherlands).Using a homogenizer, the samples were added to the deionized water to keep the concentration at 10 g/L and maintained pressure around 20,000 Pa under room temperature.www.nature.com/scientificreports/Batch adsorption.Using VWR centrifuge polypropylene tubes, 10 mL of a 200 mg/L MO solution was added to a total of 10 mg of each adsorbent (GO/CS, 1.5% PEG-GO/CS, and 2% PEG-GO/CS) and magnetically agitated at 200 rpm for 2 h at neutral pH and room temperature to determine the most effective adsorbent.
During each experiment, a certain volume of the solution was withdrawn at regular intervals and filtered using a 0.45 m membrane filter.The amount of MO was evaluated at a wavelength of 467 nm using a Perkin-Elmer Lambda 25 UV-Vis spectrophotometer (Waltham, MA, USA).To determine the percentage of removal, the following Eq.(1) was used: where C 0 (mg/L) represents the initial MO concentration, C e (mg/L) denotes the concentration at equilibrium.Based on the removal %, the 1.5% PEG-GO/CS adsorbent was selected for future investigation.It has been observed that the impact of controllable parameters on adsorption capacity was significant, and because of this, it is worthwhile to analyze it in further detail using the Taguchi analysis optimization approach.This investigation examined four factors, including contact duration, pH, adsorbent dose, and starting concentration of MO, and five different levels of each factor were tested (Table 1).In each trial, 10 mL of dye solution was stirred at 200 rpm.By periodically adding either 0.1 mol HNO 3 or 0.1 mol NaOH solutions, the pH of the solution was maintained in the desired 2-9 range.According to Table 1, adsorption studies in the batch mode were carried out at room temperature.The adsorption capacity was determined using the below Eq. ( 2): where Q e (mg/g) is the adsorption amounts at equilibrium, C e (mg/L) denotes the concentration at equilibrium, C 0 (mg/L) denotes the initial MO concentration, m (g) is the dosage of the adsorbent, and V (L) is the adsorbed solution volume.
Adsorption isotherms were examined by adding a known quantity of 1.5% PEG-GO/CS (10 mg) to 10 mL solutions of 50-250 mg/L MO in a series of conical flasks.The resultant mixture was shaken for an hour in a water bath maintained at room temperature.The solution was filtered at the end, and the resulting filtrate's MO content was measured spectrophotometrically at 467 nm.
The batch adsorption studies were performed in a series of conical flasks, allowing for the measurement of the adsorption process' kinetic characteristics.At a pH of 2, each flask has 10 mL of MO solution (200 mg/L) and 10 mg of adsorbent in it.Each flask's contents were agitated in a shaker bath at room temperature for a fixed amount of time.After that, the shaker was turned off, and the flasks were filtered.Absorbance measurements at 467 nm were used to determine the remaining MO concentration in the filtrate after the process.Adsorption capabilities were determined at various times and then fit into kinetic models.
An aqueous solution of 200 mg/L MO dye and varying concentrations of NaCl (0.1-0.5 M) was used to study the impact of ionic strength on the adsorption capacity of MO.To carry out the regeneration test, 10 mg of adsorbent was added to 10 mL MO solutions (200 mg/L) in a conical tube.The adsorbent was separated, rinsed with distilled water, and placed in a 50 mL conical tube after 2 h of agitation at 200 rpm.After the addition of 10 mL of the 0.05 M NaOH, the mixture was agitated for 2 h.The adsorbent was removed, washed, neutralized, and reintroduced to the fresh MO solution before being removed, washed, and neutralized.In order to test the produced adsorbent's reusability, three cycles of regeneration and reuse were performed.

Results and discussion
Characterization.The application of functionalization would profoundly change the substrate material's form and the fundamental characteristics of its surfaces.We examined the surface characteristics and interfacial interactions of GO/CS and the GO/CS/PEG composites using SEM and TEM images.As seen in Fig. 2a,d, the surface of the GO becomes rougher after being grafted with CS, indicating the GO's crosslinking or tangling with CS.The GO sheets are disseminated in the chitosan matrix in a unidirectional manner parallel to the composite (Shadow of the thin film).Establishing amide connections between GO and chitosan can make it easier to disperse GO throughout the chitosan matrix 25 .The subsequent PEG-modified GO/CS composite surface results in an even greater surface roughness increase (Fig. 2b,e).A 3D network structure was formed when the molecular chain of PEG was incorporated, which might further decrease the van der Waals force between molecules and enhance the dispersion of GO 26 .Additionally, as can be observed in Fig. 2c,f, the PEG-GO/CS composite structure is more fracture and irregular due to the higher concentration.Overall, according to SEM and TEM analysis, 1.5% PEG-GO/CS sample is accompanied by distinctive morphology with a more stable surface, which is advantageous for applications involving the trapping of dye substances.
The interaction of functional groups between GO/CS and GO/CS/PEG composites was investigated using a Fourier transform infrared spectroscopy (FTIR), and the spectra are presented in Fig. 3a.The FTIR spectra of GO/CS reveal the combination characteristics of pure graphene oxide and chitosan, which includes the broad peak at 3424 cm −1 corresponding to the mixture of amine stretch (CS) and OH groups (GO).Next, the peak at 1688 cm −1 demonstrates the existence of COOH groups derived from graphene oxide, which is moved lower due to hydrogen bonding between GO and the hexatomic ring of CS 27 .The peak at 1528 cm −1 certifies C=C groups in GO, indicating the existence of N-H bonding due to the presence of CS.The peak around 1098 cm −1 due to C-O-C stretching can be associated with GO layers.Most importantly, the amide interaction between the carboxylic in GO and NH 2 groups in CS is shown by the disappearance of the carboxylic acid peak 28 at 1731 cm −1 .The data suggested that GO and CS interacted with one another.The FTIR spectra of PEG-GO/CS displayed considerable similarities to those of GO/CS and PEG, and To that end, the PEG modifier is characterized by a set of spectral features, including stretching vibrations (C-H) at 2960-2880 cm −1 and stretching (C-O-C) found between 1250-1030 cm −1 .Moreover, the OH groups stretching of the PEG causes a strong and sharp peak at a higher wavenumber 29 of 3435 cm −1 .Besides, the peak at 1821 cm −1 generalized the ester bonding confirmation between PEG and GO/CS sheets.Finally, the 832 and 952 cm −1 peaks represent PEG's crystalline characteristics, which can demonstrate the successful composite formation of PEG-GO/CS.
Figure 3b displays the XRD patterns for GO/CS, 1.5% PEG-GO/CS, and 2% PEG-GO/CS from 10° to 80°.An amorphous structure may be inferred from the XRD pattern of GO/CS, which displays a strong peak at 2θ = 25.8°.The disappearance of the typical CS diffraction peaks and the GO diffraction peak is intriguing since it shows that the fully exfoliated arrangement of GO sheets has been established in the chitosan structure 24 .On the other hand, two peaks at 2θ = 19.48°and 2θ = 23.43°characteristic of PEG 30 can be seen as a result of PEG's integration into the GO/CS composite.When comparing the 2% PEG-GO/CS to the 1.5% PEG-GO/CS sample, it is clear that the latter has more crystallinity tuning flexibility.Overall, the crystallinity of the composite improves once PEG is added due to the high crystalline structure of PEG molecules themselves 31 .
As seen in Fig. 3c, the thermogravimetric analysis (TGA) was used to explain the thermal stability of GO/CS, 1.5% PEG-GO/CS, and 2% PEG-GO/CS.The TGA is useful for analyzing a sample's weight loss due to heating it in a certain environment.Differential thermogravimetric analysis, often known as DTG (inset of Fig. 3c), was used to identify the temperature at which the highest rate of weight loss would occur, and this value was found to be precisely the same as the breakdown temperature.Figure 3c shows that the GO/CS sample had three distinct loss phases between 50-100 °C, 150-330 °C, and 350-430 °C.This is in line with the loss of water, the breakdown of oxygenated functional groups, and the complete pyrolysis of the carbon skeleton 32 .Figure 3c shows a thermogram developed with 2% PEG-GO/CS, which is identical to GO/CS except that the beginning decomposition temperature of the composite has moved to about 180 °C and the weight loss occurring during 350-430 °C has risen from 19% (GO/CS) to 22.0% (1.5% PEG-GO/CS). Figure 3c shows that 1.5% PEG-GO/ CS degradation begins at 198 °C, with intermediate temperatures of 150-330 °C and 350-430 °C, much as GO/ CS and 2% PEG-GO/CS.Weight loss is minimal compared to GO/CS and just 2% in PEG-GO/CS degradation steps.One possible explanation is that PEG bonds with the GO/CS combination 33 .Because of the strengthened connections between the PEG and the GO/CS, the composite can withstand temperatures up to 800 °C without losing more than 30% of its initial weight.Given this increased stability, the PEG-loaded GO/CS composite seems to be a good fit for high-temperature-aided water treatment.XPS spectra verified the surface composition of 1% GO/CS, 1.5% PEG-GO/CS, and 2% PEG-GO/CS (Fig. 3d).The XPS survey spectra indicate three peaks at around 285.2 eV, 400.5 eV, and 532.7 eV, assigned to the C1s, N1 s, and O1s core levels, respectively; their narrow scan spectra are shown in Fig. S1.Table S1 provides an overview of binding energy and atomic surface concentration.According to the relative elemental analysis, the PEG-GO/ CS composite had higher oxygen and nitrogen levels than GO/CS but lower carbon content 34 .Consistent with the FTIR findings, PEG-GO/CS was highly soluble in an aqueous solution due to several hydrophilic functional groups on its surface.In producing GO/CS-PEG composites, the hydrophilic ligand, such as PEG, may play an important role.

Selection of adsorbent.
The MO was used as a model synthetic dye.The removal efficiency of several adsorbents synthesized under different circumstances was studied to determine which adsorbent was most suited for the batch tests.The relative effectiveness of several adsorbents in removing MO is shown in Fig. 4a,b.The removal efficiency of MO varies greatly amongst adsorbents.In the case of GO/CS, its MO-removal capacity is just 23%.When PEG was added to the GO/CS composite, a much higher removal of MO was found.
Regarding the 2% PEG-GO/CS ratio, the MO removal percentage was only 40%.On the other hand, 1.5% PEG-GO/CS enhanced the removal of the MO to 71%.This may be ascribed to the fact that introducing PEG at this dose offers additional adsorption sites and a higher positive surface charge (Fig. S2), leading to increased MO sorption.Therefore, we choose the 1.5% PEG-GO/CS composite for further adsorption studies.
Taguchi analysis of Qe of 1.5% PEG-GO/CS.Adsorption of MO was carried out using the L25 orthogonal experimental technique, followed by the determination of optimal sorption condition using the 1.5% PEG-GO/CS.Table 2 displays the Qe values concerning their S/N values for the adsorbed samples.In general, the more dye adsorbed as an adsorbate, the greater the Qe of the sample.Signal-to-noise (S/N) ratio assessment.The fundamental goal of Taguchi's study, which often involves the S/N ratio, was to determine the optimal environment for acquiring and analyzing the different processing parameters.The S/N ratio is used to evaluate the degree to which observed data deviates from the predicted one, where signal stands for desired values and noise for unexpected ones.There are three different S/N ratios, and for the sake of this investigation, the one with the largest sample size was chosen (Eq. 3) 35 (higher adsorption capacity).where y i is the result of the ith experiment in the orthogonal array design, and n is the total number of times the experiment was performed.Table 3 displays the response average S/N values derived at the 5 levels for the 4 factors.We also calculated delta characteristics to identify the most critical parameters by subtracting the highest and lowest average S/N ratio values from each set 36 .Then, they're assigned using a rating system where 1 represents the highest value, 2 is the next highest, 3 is the next highest, and so on.The highest delta value (12.24) was found for the initial dye concentration, making it clear that this was the most essential element.The next three most important factors were solution pH (2.67), adsorbent dose, and time, with a value of 1.45 and 0.44, respectively.In addition, the major impact plot of the process parameters for the S/N ratios (data means) in Qe of MO adsorption is shown in Fig. 5.The effect of the different process parameters may be shown by comparing the values of the separate process parameters to a solid line.If a certain process parameter is located close to the dashed line, this suggests that the process only has little impact on adsorption behavior.On the other hand, the adsorption process is predominantly influenced by a parameter with a steeper slope.Thus, among the factors that were investigated, it was found that initial dye concentration (D) and solution pH (A) had a statistically significant effect on adsorption capacity.On the other hand, adsorbent dose (C) and time (B) had a very moderate impact.Considering this, the best circumstances have been classified as A1B5C5D4, which resulted in the greatest possible Qe when the Taguchi approach was used.This is significant since the highest possible Qe signifies the most effective adsorption performance.
Interaction plots.The behavior of the levels of process parameters depends on their interaction, which can only be determined by analyzing the interaction graph.Two distinct patterns of behavior resulting from interactions are possible: parallelism and non-parallelism.The interaction effects of the input parameters may be seen by examining the plot's non-parallel and parallel lines.Parameters are highly dependent on one another for nonparallel lines but only somewhat dependent in the case of parallel lines 37,38 .Figure 6 shows the interaction plot, which shows that the three independent variables (adsorbent dose, contact time, and solution pH) have significant interactions, as shown by the non-parallel lines (three lines intersect with each other).Besides, it was  observed that the initial dye concentration (D) had non-parallel solid lines, indicating that its values were not as reliant on each other as was initially assumed, leading to the most influential parameter.Overall, analysis of interaction plots, which are very useful for analyzing process aspects, reveals that the selected parameters had a major effect on the methyl orange adsorption efficiency.

Analysis of variance (ANOVA).
After applying the Taguchi technique to the findings gained from experimental testing and the calculated S/N ratio, an ANOVA is used to determine the relative relevance of different components.The S/N ratio may be used to determine the optimum conditions in which the maximum response value is obvious.However, it cannot provide data on the central variable in the experiment, whereas ANOVA is able to exhibit the required information.In this case, the SS factors produced from trial results were initially supposed to be used to split the distribution of measurements.The proportion of MS values was utilized for F-value since it represents the most critical factor in the model.If the p-value of a factor is less than 0.05, it is deemed significant 39,40 .ANOVA results for Qe of MO are shown in Table 4.The greatest F-value found for this relationship was 152.17, with a corresponding p-value of 0.00 (significant) and an overall contribution percentage as high as 92.05% (Fig. 7), entirely attributable to the initial dye concentration.Also, the solution pH showed statistical significance (0.02) with a percentage contribution (C%) of 4.62 (Fig. 7).Moreover, the percentage contributions from adsorbent dose and contact time, respectively, were 1.39% and 0.12%, with the latter two contributing so little as to be statistically insignificant.
Analysis of residual plots.Figure 8 displays the residual plots (normal probability plot versus fits, a histogram, and versus order) for the S/N ratios of adsorption capacity (Qe).Throughout the adsorption process, residuals follow a normal distribution, as seen by the produced normal probability plot, in which most points lie on or very close to the line.A residual vs. fitted values graphic is used to determine whether the input parameters  impact the output results.This shows that the residuals have a constant variance significance 41,42 , since the spots lower in the graph are gradually horizontally oriented, while the spots higher in the graph are directed more arbitrarily toward the residual lines (zero value).The histogram bars show that the residuals only have a variance point for a small number of observations.Lastly, an examination of residuals vs. order shows that the residuals are scattered randomly with respect to the zero lines, emphasizing that they rely heavily on dye removal.
Fitted plots assessment.The regression equation allows for accurate computation and comparison of predicted values depending on experimental conditions 43 .Figure 9 displays the predicted vs. experimental responses in a fitted plot for the Qe of methyl orange.It can be seen that the experimental and predicted Qe are very well aligned, with an R 2 value of 98.2% and an adjusted R 2 of 98.1%.When there is less dispersion in the values around the mean, it is clear that the model can make an accurate prediction.The Pearson correlation between  the predicted and actual Qe was 0.9818, and the study's P-value was 0.000.There is a high correlation between the predicted and observed fixation rates, as shown by this finding 44 .
Confirmation test.The Taguchi methodology relies on a confirmation test to further validate its findings, and this test is strongly recommended for statistical procedures.The main purpose of this validation test is to confirm the reliability of the assessments and the results 45 .Table 5 displays the results of the validation tests.In order to ensure that the process has been optimized, it is necessary first to infer the ideal circumstances.The predicted values were calculated algorithmically.In light of this, the experiment was conducted using the ideal parameters, and it was found that the S/N ratio had been adequately increased.The major objective of this study was to raise the Qe (which was achieved by an increase in the S/N ratio of 0.96).These results demonstrated the efficacy of a standardized, statistical approach to experimentation in enhancing performance.

Adsorption kinetics. Adsorption kinetics as a function of contact time is an essential indicator for
determining the rate constant of the whole adsorption process 46,47 .Hence, the adsorption kinetics of MO onto 1.5% PEG-GO/CS were studied, and the findings are shown in Fig. 10.Initial adsorption rates were high but gradually decreased as the experiment progressed, eventually reaching equilibrium.Dye adsorption was shown to be rapid during the first 20 min, and equilibrium was attained after 60 min.This rapid dye removal during the first adsorption stage has been attributed to several empty sites dispersed over the composite surfaces.
Nevertheless, the dye removal rate significantly slows down in the last phase, likely owing to the significantly reduced number of empty sites on the surfaces of 1.5% PEG-GO/CS and the aggregation of these particles during adsorption.The findings show that PEG inclusion into GO/CS matrix improved adsorption performance by providing active sites for MO removal.In addition, the kinetics of adsorption were analyzed using nonlinear pseudo-first-order (PFO) (Eq.4) and pseudo-second-order (PSO) (Eq.5) models 48 .
where q t (mg/g) is the maximum amount of dye that may be adsorbed in a given amount of time, t, k 1 (min −1 ), and k 2 (g/mg/min) are the pseudo-first and pseudo-second-order kinetic rate constants, respectively.The fitted curve is shown in Fig. 10, and the corresponding fitted values are shown in Table 6.There is a clear preference for PSO kinetic model, as shown by the high coefficient of determination (R 2 = 0.9810) and the (4) q t = q e 1 − e −k 1 t (5) q t = k 2 q 2 e t 1 + k 2 q e t Figure 9. Fitted lines for the experimental S/N ratios (T%) and predicted S/N ratios (T%).presence of a good agreement between the predicted and observed qe values while analyzing the adsorption performance of MO.Besides, the PSO model presented lower average relative error (ARE) and standard deviation (SD) values 49,50 .A similar kinetics trend was reported by Liu et al. 51 and showed that the PSO model offers the best adsorption rate for methyl orange by GO-based adsorbent.Also, Huang et al. 52 accurately fitted the methyl orange adsorption kinetics by PSO in the presence of crosslinked chitosan-based adsorbent.The findings indicate that the chemisorption mechanism was the primary adsorption process 53 .This suggests a transfer or interchange of electrons between the adsorbent's binding sites and the methyl orange molecule.Notably, the adsorption rate of MO by 1.5% PEG-GO/CS was enhanced after incorporating PEG.According to the prior investigation, incorporating PEG increased methyl orange's adsorption efficacy through PEG-modified composite adsorbents 54 .
The findings of our study indicate that the utilization of the PEG ligand has the potential to augment the elevated specific surface area of the 1.5% PEG-GO/CS composite, thereby rendering it more conducive for diffusion and leading to rapid adsorption kinetics.

Adsorption isotherms.
In the process of adsorption, adsorption isotherms play a crucial role.An adsorption isotherm is formed when an adsorbate and an adsorbent are in contact with one another over a period that is long enough.There is a state of dynamic equilibrium between the adsorbate concentration at the interface and the adsorbate concentration at the solution phase 55 , leading to obtaining the maximum adsorption capacity.The Langmuir model (Eq.( 6)) and the Freundlich model (Eq.( 7)) are two well-known nonlinear isotherm models that are utilized to explore the adsorption behavior in the current work.Adsorption onto the surface of a homogeneous solid adsorbent is shown to occur as a monolayer by the Langmuir fitted model 52,53 , whereas adsorption onto the surface of a heterogeneous solid adsorbent is shown to occur as a multilayer by the Freundlich fitted isotherm model.where q max is the maximum MB adsorption capacity (mg/g), KL is the Langmuir equation constant, and Ce is the equilibrium solution concentration.The value of 1/n is used to illustrate the adsorption intensity, while the value of KF represents the Freundlich constant.Figure 11 depicts the fitted curve, while Table 7 provides the obtained isotherm parameters.The adsorption isotherms for 1.5% PEG-GO/CS showed monolayer adsorption on the homogeneous adsorbent surface, as shown by a high coefficient of determination (R 2 ) found for the Langmuir model.The Langmuir model also presented lower values of ARE and SD 56 .The adsorption isotherms for 1.5% PEG-GO/CS showed monolayer adsorption on the heterogeneous adsorbent surface, as shown by high correlation co-efficiency (R 2 ).The findings show that the 1.5% PEG-GO/CS can adsorb up to 271.00 mg/g of MO.As a larger KL of the adsorbent leads to a better adsorption performance at a low concentration 57 , this suggests that the 1.5% PEG-GO/CS significantly boosted the adsorption capacity of MO.According to Table 8, when comparing our adsorbent to other adsorbents for MO adsorption, 1.5% PEG-GO/CS has an outstanding adsorption capacity, much greater than others.This demonstrates that the 1.5% PEG-GO/CS has great potential as an ideal adsorbent for cleaning up wastewater containing MO.
Ionic strength and reusability.Wastewater from industries may comprise various pollutants, including dissolved and suspended compounds, acids or alkalis, salts, metal ions, and more.The presence of ions increases the ionic strength of a solution, which may affect adsorption efficiency 67 .NaCl was introduced to the solution at different concentrations to investigate the effect of ionic strength on the adsorption capacity of MO in the 1.5% PEG-GO/CS.The adsorption capability of MO was shown to decrease in tandem with increasing NaCl ( 6) q e = q max k L C e 1 + k L C e (7) q e = K F C e 1 n   through electrostatic attraction.On the other hand, adsorption capability falls when the pH of the MO solution rises.As the PEG-GO/functional CS's groups are deprotonated in a basic solution, the dye-uptake capacity drops along with it 72 .This is because the interaction between the PEG-GO/CS and MO is attenuated.The MO adsorption capability may decrease because the numerous OH ions compete with the MO anions for adsorption sites.Overall, it is considered that electrostatic interactions, π-π, and H-bond are mainly responsible for MO adsorption by PEG-GO/CS composite (Fig. 14) 73 .

Conclusions
This research describes the hydrothermal synthesis of a composite of graphene oxide (GO) and chitosan (CS) functionalized with polyethylene glycol (PEG) and used to remove methyl orange (MO) dye from water.The characterization studies indicated that adding PEG-tuned GO/CS composite surface structures improved sorption performance.The composite with 1.5% PEG-GO/CS exhibited a robust structure and a high removal efficiency (71%) compared to the others.The effects of solution pH, contact duration, adsorbent dose, and starting dye concentration on the dye adsorption process were studied.The L 25 Taguchi experimental design approach was used to get these ideal values for the variables above.These parameters were found to be most favorable at an initial pH of 2, a period of 90 min, an adsorbent dosage of 10 mg/10 mL, and an initial MO concentration of 200 mg/L.Compared to prior investigations, the adsorption capacity of the composite was higher at 271 mg/g, and it showed superior agreement with the pseudo-second-order kinetic model and the Langmuir isotherm.The surface charge of 1.5% PEG-GO/CS was highly positive, which may assist in improving the sorption capacity of MO from an aqueous solution.NaCl, representing ionic strength, was shown to negatively impact the adsorption capacity.The 1.5% PEG-GO/CS composites can be regenerated and reused for three consecutive cycles.The high dependence of sorption capacity on pH suggested that the electrostatic interaction was the primary driving mechanism for MO sorption.

Figure 10 .
Figure 10.Pseudo-first-order and pseudo-second-order kinetic models for the MO adsorption on 1.5% PEG-GO/CS.

Figure 13 .
Figure 13.The effect of the pH on the MO adsorption capacity and zeta potential.

Table 1 .
Selection of factors and levels in the Taguchi design.

Table 2 .
Results of MO adsorption based on L 25 Taguchi design.

Table 3 .
Response table for S/N ratios in Qe of MO adsorption.

Table 4 .
ANOVA for S/N ratios of adsorption capacity (Qe).DF the degrees of freedom, SS the sum of squares, MS the mean squares, F Fischer's test, p-value the critical probability.

Table 5 .
Results of the confirmation experiment.

Table 7 .
Adsorption isotherms parameters for MO.